Rochester Institute of Technology
RIT Scholar Works
Lusters and the slab form in raku
Follow this and additional works at:
This Thesis is brought to you for free and open access by the Thesis/Dissertation Collections at RIT Scholar Works. It has been accepted for inclusion in Theses by an authorized administrator of RIT Scholar Works. For more information, please firstname.lastname@example.org.
LUSTERS AND THE SLAB FORM IN RAKU
Richard A. Hirsch
Candidate for the Master of Fine Arts in the College of Fine and Applied Arts
of the Rochester Institute of
Advisor: Professor Hobart Cowles
Index of Slides iii
Reasons for the Investigation 1
Chapter I Trial and Error Period 4
Chapter II Further Technical Research 10
Chapter III Correlation of Lustered Glazes on Slab Forms 15
Some Observations 18
Chapter IV Continued Glaze Research 20
SLIDE LIST - RICHARD HIRSCH
1. Lusterd Plate 20 1/2"
2. Gold Luster Plate 21"
3. "Rainbow" Plate 18 1/2"
4. Footed Bowl 10" high
5. Lustered Plate 18"
6. Lustered Plate 19"
7. Bowl 9 1/2" high
8. "Landscape" Plate 20 1/2"
9. Lustered Bowl 10 1/2"
BigBowl 28 1/2"
Goblet 11" high
12. Luster Goblet 10" high
SprayLuster Goblet 12 1/2" high
14. Raku Goblet 10 1/2 high
15. Footed Goblet 12"
16. "Mother of Pearl" Goblet 15"
17. Gold Goblet 16"
18. Gold Goblet 15"
19. Crackle Bottle 10 1/2 ht.
20. Luster Bottle 8"
(Orange)21. Precious Object Box 4x4x5"
22. Object Box 4x4x5"
23. Black Box 4x4x5"
24. Gold Precious Box 5x5x5"
25. Shell Box 6x5x5"
26. Gold Coil Box 14x4x3"
27. Gold Box with
28. Raku Box 15 1/2"
29. Covered Form 21 1/2"
30. Covered Form 21" ht.
31. Covered Form 22" ht.
32. Covered Form 26"
33. Covered Form 30"
Mythesis is not one that proves a
point,nor professes to be a new break-through in ceramics.
Basically,it is a report on my involvement with Raku at The School for American Craftsmen. A major goalwas to
attain practical and usable knowledge in this particular process. The pur pose of the thesis was to correlate my investigations of lustered glazes with
slab built forms usinga Raku process. I decided to concentrate in one
area,rather than dabble in many. Trial and error seemed to be the only way to
begin to investigate and
developtechniques. This approach fit my person
ality. Pride of accomplishment was a reward for
longhours of testing. Failures were not
depressing,because in them knowledge was acquired.
inquiryled to experience and understanding. What
the involvement actually accomplished was to give me a better understand
ingof pottery in general.
Throughout my entire
learningexperience at SAC Professor Hobart
Cowles was primarily responsible for
directingmy insights and discoveries
into the Rakuprocess. More
importantly,he offered me inspiration.
-v-REASONS FOR THE INVESTIGATION
When Icame to the School for American Craftsmen my background
was limited to some cone 9 reduction stoneware.
Duringthe first few
weeks at SAC I continued with cone 9. A fewglaze tests were run, but
at the time I lacked enthusiasm.
Duringthe Rochester Clothesline Show and Sale I had seen a
displayof pottery which stimulated my interest. Strange colors made the work stand apartfrom all I had seen. The
potter only mentioned that the glazes were metallic lusters obtained
bya process known as Raku.
Included among the graduate students were Drew Krouse and John Frisenda. Both Krouse and Frisenda expressed a willingness to
tryRaku. What started out as a jointventurebecame an individual effort in self expression.
Achievement ofaesthetic goals relied
heavilyupon technical con
Duringmy investigation all elements ofa Raku process were dealtwith.
Raku,like most other forms ofpottery
sists of three main components: the
clay,the glaze, and the fire.
Onlyafter all these aspects ofpottery are understood can a person give form to his ideas.
Eventuallyaesthetic concerns dominated my thoughts after
the technical phase had been comprehended. The use of metallic lusters
Before starting the
experimentation,the many philosophies of Raku
were examined. Associated withRaku is the Oriental Zen tradition of
the tea ceremony.
byZen Buddhist philosophy, took a
unique pleasure in the conscious return to direct and primitive treatment
of clay. n1.
In accord with this is the emphasis on
beauty,the simple, and the
"The cult of tea or
Teaism,is a way of life that expresses an accep
tance and veneration of the imperfect in an attemptto imbue man'
place surroundings with great meaning and beauty. Itplaces great emphasis
on meditation and quiet contemplation as a means of
of the inherent
beautyof the non-perfectasymmetrical form. It celebrates
the excitement of surface which derives its characterfrom nature inspired
phenomena,and it becomes a part of the spontaneous creative process
transitorythough it may be. "
Until the middle fifties Raku didn't receive much attention in this country.
RecentlyAmericanpotters have made their own contribution in Raku quite
different from the strict interpretation ofJapanese potters.
Rakupots shown in the Twenty-Third Ceramic
National,a critic wrote
"Nothingwould amaze a Japanese potter more,
however,than these Raku
pots. Our style is home grown, and has little or nothing in common with
the Raku pottery ofJapan in spite of the name. uU'
Reigger,Raku: Art and
Technique,(New York: Van Nostrand Reinhold
Slivka,"The Twenty-third Ceramic
(New York: American Craftsmen's
-2-Daniel Rhodes feels "The original meaning of Rakuhas almost been forgotten.
The more immediate response from the fire has speeded up the process of
pottery making and brought a new excitement to it. " * While I considered
the ideals of the Japanese
potters,the decision was made not to use Raku
traditionally,but to seek my own
forms,and experiment without the restric
tions the Tea-Zen
philosophywould impose. After some investigationand
involvement,a personal concept would develop.
TRIAL AND ERROR PERIOD
The investigation began simply
byreadingwhat a Raku process was. Charles
describesit "as a Japanese technique
application of low
porous,low biscuit fired
pieces,and placing of the
directlyinto a pre
heated red hot
Rhodes says that Raku is a procedure rather than a specific color or
effect. "In making raku, the pottery is bisqued in the usualway, but in the glaze fire it is
directlyin the red hot
kiln,then with drawn and rapidly cooled as soon as the glaze has melted. In
firing,one or two pots are placed in the kilnwith tongs. The pots are observed through a
spy hole and whenthe glazes are smooth and
shiney,the pots are drawn out with the tongs. The glaze
firingusually takes about ten minutes. ""
Most sources researched felt that lead base glazes were the best to use because
theymelted smoothly and rapidly. ELeach notes that all the glazes of
the traditional Red Raku and Black Raku were lead
Armed with this knowledge itwas decided to fire at once! A
loading-kilnwas built out of soft
firebrick.Burners were made from plumbing
supplies,and propane gas was used as the fuel. Several lead
basedglazes were mixed and applied to the ware. After
glazed,all were placed
directlyinto the hot kiln and the gas pressure was turned up. What
followed was a comedy of errors! From then on Iknew that
were just as important in this process as in any other method or
Pottery,Iowa: (W. M. BrownCo.,
1.Glaze exploded off the pot when placed in the red hot kiln.
2. Glaze melted and ran off the ware if slightly over-fired.
3. The glaze surface was pitted and scarred fromthe combustible material.
4. Some glazes were melted while others were still immature onthe same
5. The clay
odycracked when placed in the hotkiln.
In addition to these technical difficulties there was no control over the
smoking or reducing aspects of the process. Some pots were smoked
black,while others received little smoke. Ih a few cases, halfof the pot was re
duced,while the other remained unaffected. The use ofa
was dangerous and clumsy when unloading the hot ware with tongs.
There was nobeginner 's luck and the same awful results continued in
firings.For the first time in my short involvement with
there was a desire and a need to do some technical experimentation. I
lookingfor the reasons that contribute to the failures.
bodyfirst used was a regular cone 9 stoneware.
Cedar Heights Redart 1
XX Sagger 1
bodycouldn't withstand the tremendous thermal
shock. Raku clay formulas need sufficient non-clay material to lessen the
contraction in the rapid
heatingand cooling cycles..
sand added to the clay
keepthe pores of the clay open and allow moisture
escape,preventing cracks and explosions.
one-third non-plastic material added to awhite clay recipe. To comply with these needs the
followingclay recipe was used.
North American Fire
Cedar Heights Goldart 120
The only problem was to find what temperature to biscuit fire. At
first cone 04was tried and the results were disastrous.
into the kiln exploded or cracked before the
firingcycle was completed.
Next it was biscuited at cone
08,and this temperature seemed satisfactory,
enough,yet not too brittle.
disappointingwas the poor result obtained from the lead base
Theyproduced some uninteresting
browns,garish oranges, weak
blues,also a dull galena when
heavilyreduced. Some lead
glazes thatwere tried:
White lead 60
Frit 25 20
Tin Oxide 3
White lead 60
Frit 25 40
Lead chromate 4
Frit 529 70
Soda Ash 10
Copper carbonate 3
White lead 60
Frit 529 20
Red Iron oxide 4
Copper carbonate 2
-6-Most of these lead glazes melted and ran off the ware even if slightly
over fired. Color burnt out quickly in the short
firingrange. While lead
glazes have a nice smooth
theyremain soft and set up very slowly. This resulted in a poor surface qualitywhen sawdust pitted and scarred the
soft glaze surface. High lead glazes are easily reduced, yet a
scum developes if over-reduced. Some luster was produced
but because of the reasons stated and the fact that lead is extremely
other kinds of low
firingglazes were investigated.
Ihad acquired a list of alkaline glazes that Paul Soldner is reputed to
use. I experimented with the
Burnt Umber 20
Yellow Ochre 20
Red Iron oxide 10
Copper carbonate 5
These glazes melted at ahigher temperature than the lead bases. Their
soft,less pitting and scarring occurred. Glass Red was most successful. When
duced a reddish copper; if left to air cool, it remained copper green.
-7-Traditionally,the Japanese do not smoke or reduce their Raku ware
outside of the
However,in America it is the most important part of
the process. It is the critical
point,the "make or break" step in the en
tire process. Practical experience had no substitute and control was
gained with time.
Combustible materials such as
leaves,pine needles, sawdust, news
straw,are used to create an atmosphere
lackingin oxygen and
containing free carbon.
Potterysubjected to this atmosphere undergoes
a chemical change.
Clay,as well as
Onlyon the sur
face does this change occur because of the short reducing time and low
temperature. Reoxidation ofthe glazes will take place ifthe ware is taken
out of this reducing
atmosphere,while still hot enough to effect a chemical
timingis most important. Surfaces which are
the hottest will reduce the
best.Pots should be removed from the hot
kiln and placed in the reducing atmosphere immediately. When I talked
to Paul Soldner at Geneseo last
21, 1970,he said that "a good
quick reduction is criticalfor the development of
the ware to the reducingatmosphere, a main concern is not to scar the
Heavyreductiondoesn't always depend on direct contact
with the combustible material.
Onlya reducing atmosphere is necessary.
Coolingshould be done slowly and the pot should notbe removed fromthe
reducingchamber until a chemical change can no longer occur.
Contained:in these few hurried minutes is the entire Zenphilosophy
of Raku. Reliance upon nature in the form of fire and smoke is the;essence
Duringthis dramatic period a "feel" for the captivating process
developes. The romantic nature ofthe whole process is realized.
"What remains is a philosophy or a state of mind that for me places
emphasis on the
discoveryof things notplanned. "'
Four months had gone
byand many individual techniques weredevelpoed.
Ware was glazed days in advance to allowfor complete drying. Kiln cham
bers were cooled down considerably before the next cycle ofpots were intro
duced.Sometimes only one pot at a time was fired in order to get maximum
results. Less and less combustible material was used in the smoking stage.
Unexpected and accidental effects were taken into consideration and a certain
control was obtained
bypractical experience and knowledge of the entire pro
Still,the development of metallic luster glazes had not yet been realized.
Also,the forms were not inaccord with the spontaneity of Raku. There was
evidence of a need for more technical research and aesthetic considerations.
Glaze effects in Raku are dependentupon manyvariable conditions,
byits own nature, has certain elements impossible to con
trol. Most glazes never fire exactly the same, although some colors and
effects canbe controlled and repeated.
However,because of the process,
with its margin of so called
"happenings",absolute duplication is impossible.
Individual techniques result in different effects.
time,very few of the glazes experimented.with produced the
Now,the formulation of my own glazes was necessary to
produce the kind I wanted.
I first experimentedwith copper. A saturated amount was first be
lieved to cause some glazes to
developa metallic luster. The copper was
added to this base glaze which I acquired from Robert
student at S. A. C.
Base C. M.
Frit P-25 43.6
Frit 3134 26.3
Lithium carbonate 9.9
Copper carbonatewas added to the base in these percentages: 5%-25%.
Unfortunately,because there was so much copper, it reoxidized
thus producing a very dense green to greenish black. No metallic lusters
were attained except where
Duringthe next series
tests,Red Copper oxide was used. This form of copper is already partially
reduced, and although it mixes poorlywith water and other
were better. It seemed to luster more successfully.
At this time I realized the difference in results using two kinds of
Usinga gas kiln produced better lusters from copper than an electric
In a gas kiln there is a slight reducing atmosphere in the
developthe metallic luster even before it is removed fromthe kiln.
Less Red Copper oxide in the glaze was needed to produce metallic lusters.
Inquirywas now made as to what other ceramic chemicals beside the copper
developluster. Literature on metallic lusters revealed that lusters were
a type of decoration used for centuries. Lusters were employed as a final deco
ration rather than as a complete glaze.
Historically,the development of metallic
lusters is credited to the Islamic potters. Persian ceramicists used luster as a
purely decorative media. Itwas employed in a final
alkaline glaze. These wares are reputed to be the culmination of the art of
over-glaze luster. I saw a few examples in the Royal Ontario Museum in
Describingthis form of
decoration,one source states that "Luster constitutes
a form of decoration on ceramics and glass consisting of extremely thin films of
metal which are deposited on the surface ofthe ware. " Hainbach classifies lusters
beingeither colored or colorless and their preparation
method. ^' The most expensive of these lusters are what he calls "The Noble
For the preparation of these over-glaze
lusters,a metallic salt is combined
with pine resin and lavander oil. In this method
duringan oxidizing fire to red
bythe resin and oil reduces the metallic salt, which is depos
ited onthe glaze surface.
Shaw,Ceramic Colors and
PotteryDecorations (New York: Frederick
Praeger., 1968),p. 80.
Pottery Decorating,(London: Scott Greenwood and Son.
11-Preparation of these kinds of lusters entails complicated formulas
and procedures. Expensive materials are used in the "noble metal
such as gold and platinum. Lusters developed inthese manners are now,
souvenir,ornamentalware and are used in
bandingcommon mass-produced dinnerware. Luster solutions ofthis type
are sold commercially. Most are expensive and produce a flat luster. De
veloping lusters of this quality was not my intention.
However,the use of the
chemical compounds such as the metallic salts, were investigated and
adapted to my Raku technique.
A partial list of metallic salts generally associated"
lusters was acquired.
1. Silver Nitrate
2. Bismuth Sub-nitrate
3. Gold Chloride
4. Ferric Chloride
5. Zinc Acetate
6. Tin Chloride
In addition to these metallic salts, other metallic compounds were
tested. All the metallic colorants were added to the C. M.
put through a Raku process
includingthe smokingor reducingphase.
bythemselves or in combination. Within the
followingchemicals were added to the base.
1. Cobalt Carbonate
2. Cobalt oxide
3. Chromium oxide
4.Red Iron oxide
5. Iron Chromate
6. Nickel oxide
7. Manganese dioxide
8. Tungstic acid
9. Sodium uranate
10. Potassium dichromate
those,a few metallic sulfates were tried with the same
With the exception of Copper
Sulfate,none of these developed any
Finally,I began to experiment with some ofthe me
tallic salts used in the over-glaze luster preparations. At this time a
new base glaze was
beingtested and all the salts were added
Soda Ash 44. 2
Frit W-15 30.9
Flint 65. 0
All the tests were done with a Raku process
stage. Silver Nitrate was added to the C base in 1-2%. Itproduced an
ivoryto yellowish luster. Bismuth Sub-nitrate alone produced a pearly
metallic luster. When combined with Silver Nitrate the results were quite
satisfactory. A golden luster was developed with
1%Silver Nitrate and
Bismuth Sub-nitrate in the C base. At its best this glaze was yellowish
gold in color alongwith a purple irridescence.
modulation and the Bismuth developed the over-all irridescence. (For
awhile people inthe shop called me "Beatrice" because of this glaze!)
Bismuth Sub-nitrate was also tried with Red Copper oxide. It im
parted an irridescence to the copper luster and helped as a stabilizer
to preventthe copper from reoxidizing. The result was a glaze that pro
duced every metallic color imaginable from copper. (See Slides
These two glazes were my standard in the investigation.
Soda Ash 44. 2
Frit W-15 30.9
Flint 65. 0
Alongwith these two luster glazes a vitreous englobe was developed.
Tennessee #5 Ball
Frit 3191 25
Red Iron oxide
LUSTERED GLAZES ON SLAB FORMS
Development of these luster glazes led me to seekforms that would
first,shapes became test tiles for the new glazes.
After some involvement the forms became as significantas the glazes.
Technical aspects of the Raku process also influenced the form. Ware
made in a single piece had a better chance of surviving the glaze firing.
Glazes reoxidized easily on large verticalforms. The major disadvantage
of working with these types of forms was that
theywere hard to maneuver
Large,round shapes had an even greater
tendencyto roll off
the tongs unless grabbed exactly in the middle. This was one of the rea
sons I tended to avoid
large,round shapes. Size had only reasonable
limitations,once the process was comprehended and
facilitywith the tongs acquired.
Clayslabs were investigated to create forms not associated withthose
of stoneware. Slab forms related to the Raku process and
lent themselves to many of the philosophies of Raku.
The investigation was an attempt to correlate the asymmetrical slab
formwith the excitement of surface, supplied
bythe metallic luster glazes
and the Raku process.
Slab forms were developed in series. After most possibilities were
exhausted,a new, related sequence was begun.
quality of clay and glaze was ofprimary importance to me. A surface
quality was achieved
bythe juxtaposition of shiney metallic glazes and the
dull mattness of the smoked claybody. Soft and malleable clay slabs could
impressed,and joined to create form and texture. With gentle urging and good
timingthe clay slab could
-15-be shaped using its vitality to give the form a visual strength.
The procedure was to roll out clay slabs on either
Each series used somekind of armature or basic form to support the wet
clay. Molds were made from-metal
casts. Soft clay slabs were draped on or in the molds or wrapped around
tubular shapes. Sometimes clay slabs were rolled inside cardboard boxes.
Qualities inherent in the wet clay were guided and controlled. Organic and
natural tendencies of soft clay slabs were utilized and encouraged because
itwas part of my philosophy of Raku. Forms were created
tion and modification rather than force. I tended to work with
forms in order for my work to be disassociated from the small scale of the
traditional Japanese Raku.
Glaze was almost always applied
bypouringor dipping. At
forms were entirely covered with glaze. Perhaps it was because Iwas so
Eventually,less and less glaze was used. The
bodybecame an important "negative space". These areas
were treated like negative space in painting and consideration of their final
shape was important.
The large slab plates and bowls were solely dependent upon the inter
action of glaze and bare clay. Large pools of raw glaze were poured into
the platters, and gently rolled around. When
fired,this produced large
modulating colorfields of metallic lusters.
negative space of the unglazed clay body. (See Slides :
The goblet series was the best in the use of the slab as a soft malleable
form. The luster glazes were used decoratively. Although the goblets had
some thrown elements the treatment of the slab was
same treatmentproceeded to the next series of covered
As the forms became more
independent,glaze was used to describe
them,rather than to dominate. With the large covered forms glaze was
used to visually separate the
topfromthe rest of the form. (See Slides
16-Shineyglaze zones were employed to contrast with the blackness of the
unglazed,smoked areas. (See Slides
32)Detailed brushwork seemed
unnecessary since the glazes
bythemselves were intricate enough.
Eachkind of form required special smoking techniques. The
smoke,along with the size and shape of the
piece,were factors in devel
oping certain methods.
Initially,pine needles and grasses were used.
duced some nice effects.
However,sawdust was more readily available
and it proved to be easier to control.
To prevent pittingand scarring from direct contactwith sawdust on
surface,the plates and bowls were turned over. Sawdust was
thrown on the unglazed area. A large metal dome was then placed over
the ware. It created a reducing
atmosphere,contained the smoke, and
With the goblets and small
boxes,a little mound of shredded paper
or sawdust was made. The red hot piece was placed in the center of the
smallheap. A short can or barrel was thenplaced over the ware to con
tinue the reducing process.
Most difficult to smoke and control were the large covered forms.
Smoke patterns broke up theverticality and destroyed the visual impact.
A monochromatic tone in the unglazed areas was needed to describe the
form. Best results were achieved when a clay sewer pipe was used.
Sawdust waspacked around the form after it was placed inside the pipe.
This wedged the combustible material between the form and the inside
of the pipe.
"Craftsmen of all times have battled with the material
with the difficulties of the
techniques,with the problems ofform and expres
sion. While in more primitive times the main difficulties
in our times of technical advancement the real problems lie almost wholly in
form and expression. "h).
Throughout my short experience with pottery, aesthetic concerns have
always been important.
Clayseems to be for me the best material for com
munication. "I consider clay tobe just another art media. Each artist
mustbe responsible for any ultimate value it may have. n11*
With Raku there has been a complete interaction between the material,
the fire and myself.
Individuality,which we all seek, is inherent inthe
Hand-buildingfurthers the uniqueness of each piece. A feel
ingfor each pot is acquired through the
immediacyof the process. Due in
part to this I have been interested and influenced
bythe idea of the object.
Creatingunique objects is not an original thought.
todayit is the
Manyshows inthe past fewyears have tried to restore to the object
its intrinsic value and power. Shows such as "Objects U. S. A. "
Tea and Other Cups"
have influenced my ideas rather than any individual.
"The contemporary American Craftsman is less
function,the reality of machine made
commodities,as he is obsessed
the nature of his materials and
himself,and the degree to which he can
Invitational,"A Catalogue for an
Art," Craft Horizons (New York: American Craftsmen's
-18-When my work is successful the objects have an intrinsic value,
Theytake ona precious nature, in that
a personusing them becomes more aware ofthe function
and more conscious ofthe objects themselves. In our
it is nice to know some objects are
"The Rakuware of the Zen tea masters still shows us into its spiri
tual orbit to this very
trulymade for itself has the power
to renew itself in the
energies,memories and actions of men."
CONTINUED GLAZE RESEARCH
Work continued on glazes while slab forms developed. Other chem
traditionallyused in overglaze luster were researched
Chloride,whenused in complex luster preparations, produces
a famous color called "Purple of Cassius". When added to my C base
and fired in
Raku,it yields some incredible and exotic colors. Three
hundredths of apercent of gold chloride added to the base glaze produced
shades of strawberry red with tinges of a purple opalescence. Unfortu
gold,chloride, because of its
in limited experimentation.
(Theydon't even stock it in the
testingferric chloride and stannous chloride a newkind of
technique was developed. Neither compound developed any noticeable
luster when added
directlyto the C base. A second step was to mix a weak solution of the metallic salt with sawdust. Whenthe hot piece hit
the sawdust a light
However,again no noticeable
luster was achieved. Both compounds are mentioned in connection with
"Glass surfaces, when heated and placed in contact with a metal salt
invapor form or in an atomized spray of the salt
adherent layer of an oxide ofthe metal is formed onthe glass or ceramic
surface. The thickness of the irridized film may be gauged
ent color of the light reflected from it. This succession of colors is
analogous to the wellknown Newton rings. " *
-20-Myprocedure was to glaze the ware and fire it up to temperature.
Just before the glaze
hot,saturated solution of the metallic
salt was prepared. A fine spray was directed onto the pot
after it was pulled fromthe hotkiln. The spray gun was held about six
inches from the piece. After spraying the
pot,it was either air cooled
or smoked in a sawdust barrel.
Glaze effects produced
bythis technique are difficult to describe
definingthe terms luster and irridescence.
Luster means "1. a glow of reflected light: gloss or sheen. 2. the
appearance ofthe surface of a mineral as affected
byor dependent upon
peculiarities of its reflecting qualities. " ' Luster implies a shiney
surface that may or may not be irridescent.
Irridescence implies a quality of surface that shows more than one
color as in a prism.
Bydefinition irridescence is "a showing of many
colors that are constantly changing." An irridescent surface can be
shiney, but not always. Another termoften used for irridescence is
"Mother of Pearl."
Aside fromthe differences in
terminology,the results were desirable
and the method exciting and rewarding. As yet, allthe possibilities have
not been reached. Experimentation will continue after this paper is written.
Sprayingthe soluble salts provided me with an element of control.
Areas where luster or irridescence was desired received the spray. Sec
tions not in contact with the spray remained uneffected. I could control
the amount of luster or irridescence on a given surface. Both the glaze
surface and the raw clay
Usuallya light spray produced the best results. A
^5Webster's Third International
Dictionary,3rd ed. 1965
16Webster's New World
Dictionary,elem. ed. 1961
-21-really an overload of the metallic substance. The result was often a
surface devoid of irridescence or luster. With the spray gun method
maximum control could be attained. With
fuminginside a kiln chamber,
there was more of a chance factor. The possibility everything would get
lusteringvapor did not appeal to me because these effects
enhance,the appearance of the ware. A great
variety of glaze effects could be acquired
bythe use of different colorants
in a base glaze along with different metallic salt sprays. Glazes of great
depth were achieved
Cracklingthe glaze created another variation. This was done after
the red hot pot was sprayed with the metallic salt. It was placed in a
sawdust barrel to smoke.
Periodicallythe pot was removed from the
barrel and moved about in the cool air. Sometimes a spray of cold water
caused the glaze to crackle.
Finally,the piece was left inside the smok
ingatmosphere to letthe smoke
developin the glaze crackle.
Temperature is an importantfactor in the spray technique. Most
chemicals tested did not work within the Raku heat range (1800
low). These compounds fused to the glaze surface but only produced
Meltingpoints of the metallic salts provide some clue as to whether
theymight work withinthe Raku temperature range.
cases, less temperature was needed to produce desireable results. Par
ticularlywith stannous chloride, if the surface of the glaze was too
it justvolatilized and left the glaze unaffected.
chemicals thatworked well alone were less successfulwhen combined.
The combination seemed to cancel out most
identifyingtraits of each
separate metallic salt.
Dr. Fred A.
Elder,Assistant Professor of
Chemistry,at the Roofa?^
ester Institue of
Technology,calls this deposit ofmetallic compound a
"Thin film Phenomena".
-22-Metallic solutions are either chemically or mechanically bonded to
the surface ofthe glaze. A mechanical bond is caused
in a chemical
bond,there is a reaction betweenan. acid and a base. The
metallic salt spray is the acid while the glaze is the base. Dr. Elder
feels that most metallic salts would
developan irridescence if the film
deposited was thin enough. He defines irridescence as "Interference
Patterns of Light". Absolute control of the spray solution would be nec
essary to obtain a thin enough film in order for some chemical compounds
developan irridescence. He related the idea ofvacuum plating metals
on a ceramic surface that was
totallyclean and smooth.
that different kiln atmospheres might produce distinctive changes in the
effects of metallic salts. Atmospheres of nitrogen and argon have been
investigation,the most successful of the metallic salts
were in chloride
form.The actual reason for this is somewhat of a
mystery. Dr. Elder believes that hydrochloric acid produced
chlorides is stronger than other acids such as nitric acid produced
the nitrates. Professor Cowles feels that hydrochloric acid fromthe
metallic chloride etches the glaze surface when the spray hits the hot
glaze surface, producing a chemical as well as a mechanicalbond.
With chlorides no oxygen is introduced to the glaze surface. Nitrates
contain oxygen, and produce the metal in its oxide formwhen the spray
solution is deposited onthe glaze surface.
Inhalation of these compounds is extremely dangerous because of
their toxicity. Care was taken when spraying and use of a strongven
tilation system was necessary.
Usingthe methods described in the spray
icals did not work within the Raku temperature range or atmospheric
1. Cobalt Chloride
2. Nickel Chloride
-23-3, Manganese Chloride 4. Barium Chloride
5. Zinc Nitrate
6. Ferric Nitrate 7. Aluminum Nitrate
8. Chromium Nitrate
9. Barium Nitrate 10. Strontium Nitrate
12. Molybolic Acid 13. Tungstic Acid
14. Potassium Chrom Alum
15. Cobalt Sulfate 16. Nickel Sulfate
18. Cadmium Nitrate
followingcompounds have worked withinthe Raku heat range and
atmospheric conditions using the spray technique:
1. Tin Chloride
2. Zinc Acetate
3. Ferric Chloride 4. Zinc Chloride
5. Cuprous Chloride
6. Cupric Acetate 7. Cupric Nitrate
Tin Chloride gave a glossy irridescence. Over a white base glaze it
produced a handsome "Mother of
Pearl",extremely rich in depth and
variation. The glaze used with TinChloride melted at a lower tempera
ture,thus preventingthe tin from completely volatilizing.
P. White Glaze
Frit P-25 36
Frit 3124 28
Lithium Carbonate 8
Zinc Acetate produced an
irridescent,rainbow effect and was used over
blue and green glazes. The main difference between Zinc Acetate and Tin
-24-Chloride was that the zinc produced a mat surface, while the tin was very
Ferric Chloride was the only compound tested that produced both an
irridescence and a
luster.The luster color range was yellow orange to
reddishbrown. (See Slide
20)Ferric Chloride produced an extremely
surface,which in some cases destroyed the color of the glaze be
neath. Sometimes it completely obscured the base glaze as in the case
with this glaze:
Ceramic Color and Chemical Mfg. Co., Inc. SpecialFrit 441 100
Ceramic Color and Chemical Mfg. Co., Inc. Red Stain 3352 7
If Ferric Chloride was sprayed on
thicklythere was a noticeable build
up of iron. This thin deposit was brown in color and devoid of any luster
or irridescence. Best results were gottenwhen Ferric Chloride was used
over the clear and the yellow base glaze.
Soda Ash 74
Frit W-15 310
Usingthe yellow glaze underneath the Ferric Chloride
range was yellow to red orange. Both had luster and irridescence.
Alongwiththese metallic compounds some soluble salts of copper were
Actually,the spray just deposited the metal substance on the glaze
surface. Ifleft to air cool, the copper would stay a familiar green. Reduc
tion was necessary to produce a metallic luster. A copper yellowwas
bythe spray method.
MeltingPoints of some chemical compounds
AntimonyChloride 73.4C 220.2
Barium Chloride 925 1560
Bismuth Sub-Nitrate 260 ,
-Cadmium Chloride 568 960
-Cupric Chloride 498
-Cuprous Chloride 422 1366
Cupric Nitrate 114. 5
-Ferric Chloride 282 315
Manganese Chloride 650 1190
Molybdium Chloride -
Platinum Chloride 581
-Selenium Chloride - 288
Silver Nitrate 212 444
Silver Chloride 455 1550
Stannous Chloride 246.8 623
Tungstic Acid 1473
Ihave heard Raku described as
beingquick and flamboyant.
believe it is a fad soon to vanish from the American ceramic scene. Others
feel it is a valid use of ceramic materials. Some say Raku depends too
much on luck. While Iwill admit there is a certain amount of luck
I submit that this is true in many ceramic processes on the studio leveL
culture,we may be
sure,divine power has been involked
for the success of the
gods,prayer sticks, and offerings
have been common.
Placingone's pieces in the kiln is 9,kind of surrender,
a givingup to the metamorphic forces of the fire."17. "The greatest pots
are those one meets coming fromthe kiln as strange objects;
seem, in texture and
color,quite beyond one's power to visualize or pre
America,the term Raku will fade into the background.
Hopefullythis pottery willbe given merit for what it looks like rather than
slighted for how it is made.
For the past two years I have worked almost exclusively
luster glazes on slab forms.
Manytechniques were developed using a Raku
Myenthusiasm for the process is still undiminished and further
exploration will continue.
"Raku,which was originally an aspect of a Zen-inspired tea
become a vehicle for the sudden thrust of intuition and the playingof hunches:
the power of Zen still at
With Raku I have been able to understand more
intimatelythe power of
fire as it transforms clay and raw chemicals into ceramic objects.
Earhart,W. H. and
Koenig,J. H., Literature Abstracts of Ceramic
Florida: College Offset
Pottery Decorating,London: Scott Greenwood and
Pottery,Iowa: W. M. Brown Co. , 1968.
Invitational,A Catalogue to an
Reigger, Hal,Raku: Art and
Technique,New York: Van Nostrand Reinhold
Clayand Glazzes for the
Potter,Philadelphia: Chilton Book
Sanders,Herbert H. , The World ofJapanese
Shaw, Kenneth,Ceramic Colors and
Pottery Decoration,New York: Fred
Rose,"The Twenty-third Ceramic
Craft Horizans (Jan
, "The Object:
Webster's New World
-28-Webster's Third NewInternational
Dictionary,3rd ed. , 1965.
Marguerite,Pottery: Form and
MADE IN U.S.A.
vsn NI 3QVW